a-Si:H 0.35 µm a-Si:H 0.02 µm a-Si:H 1.5 µm ZnO 1 µm Al 50 µm polyimide substrate
Fig. 3. Solant VI prototype (42 x 9.6 x 1.1 cm)
Fig. 2. Structure of the a-Si:H solar cells (not to scale) Characteristics of the solar module (terrestrial STC, 2 100 mW/cm , 25°C, AM1.5 spectrum): Voc AM1.5 = 9.94 V, Isc AM1.5 = 165 mA, FFAM1.5 = 50 %. At the maximum power point (MPP) a current of 122 mA was measured at 7.0 Volts (821 mW). We have calculated the characteristics of 2 the module for typical space conditions (135 mW/cm , 70°C, AM0 spectrum). We have obtained the following values: Voc AM0 = 9.19 V, Isc AM0 = 208 mA, FFAM0 = 47 %. This results in a power of 899 mW at the MPP for space conditions, power which is by far enough to supply the amplifier integrated on the back of the antenna. Characteristics of the antenna: 6x1 elements phased array working at 3.85 GHz. The beam is tilted of 15°. The circularly polarized single element consists of a cross slot excited with a single line. An MMIC amplifier is integrated in the antenna. The antenna gain is 11 dBi (passive) and 31 dBi with the MMIC. Concept of integration: The ground plane (with the slot crosses) of the antenna is printed on the antenna substrate, and then the solar cells modules are glued on it. In the breadboard, two solar modules base units are connected in parallel and three such pairs in series.
RADIATION HARDNESS OF THIN-FILM SILICON SOLAR CELLS FOR SPACE APPLICATIONS Solar cells in space are highly exposed to proton radiations. It has been shown recently that CIS  and thin-film amorphous silicon [4-7] solar cells have good radiation hardness com pared to conventional Si and GaAs devices. The µ power/weight ratio of thin-film solar cells is very promising for space applications, where
weight is an important cost factor. Thin-film double junction solar cells using amorphous silicon (a-Si:H) and micro-crystalline silicon (µc-Si:H), i.e. so called "micromorph" tandem Fig. 4. Cross section of double junction p-i-n micromorph (a-Si:H/µc-Si:H) solar cell
cells [8-10] could be a promising candidate for satellites but their radiation hardness was so far not known. A series of irradiation experiments was therefore conducted. Our test samples are thin film n-i-p amorphous and p-i-n micromorph silicon solar cells deposited on different types of substrates. The structure of the micromorph devices is illustrated in Fig 4. All the devices were manufactured by the Very High Frequency Glow-Discharge (VHF-GD) technique  at IMT Neuchâtel. Prior to starting the irradiation process, all cells were annealed at 180°C for 90 minutes. The pre-irradiation conversion efficiency was between 7.5 and 8.5 % for the a-Si:H cells and between 10 and 11 % for the micromorph cells. Our solar cells were irradiated by the European Space Agency (ESA) at CEA (Paris). All cells were irradiated under open-circuit conditions, for the a-Si:H through the front side (p-side) and for the p-i-n micromorph cells through the back side (n2-side). The 2 fluence (quantity of particles per area) was 1.5E13 p+/cm . The energy spectrum of the incident protons is shown in Fig. 5. 5.0
% ! %
$ [email protected] 7 # < = BC A "
4.0 % of incident protons
For the n-i-p amorphous silicon solar cells (on polyimide, stainless steel sheet-metal and glass substrates), the results show that these cells are only very slightly damaged by proton irradiation at the chosen fluence and energy. The efficiency loss is only a few percent (3 - 5%), and it is immediately recovered by annealing at 100°C. For the micromorph solar cells (on glass substrates), all three parameters show an important loss after the proton irradiation. Fig. 6 presents normalized efficiency of p-i-n micromorph solar cells on glass substrates after proton irradiation and after subsequent annealing at different temperatures (100°C for 5 hours, 140°C for 2 hours, 180°C for 2 hours). Experimental results of two different samples are illustrated. The degradation induced by the proton irradiation could be almost completely recovered with the post-irradiation annealing steps.
1.0 0.0 0.1
Transmitted proton Energy (MeV)
Fig. 5. Energy spectrum of the incident protons Compared to the typical irradiation energy of 10 MeV, the spectrum is shifted to lower energies, which are potentially more harmful for thin-film solar cells. After irradiation, annealing steps at increasing temperatures have been carried out. The cells were characterized before and after irradiation, and after the post-irradiation annealing steps. This was done at the IMT with a solar simulator under 2 AM1.5 conditions (1000 W/m , standard terrestrial conditions STC) and with spectral response measurements. Three parameters were measured: the open circuit voltage (Voc), the short circuit current (Isc), and the fill factor (FF). A fourth parameter is calculated: the efficiency (η). The difference for AM0 (space) 2 conditions (illumination in space: 1360 W/m ) would be an increase by 22 % of Isc, and a small reduction of FF and η. Comparisons are made w.r.t. the mean value of the normalized conversion efficiency of six cells from the same substrate for each sample.
1 D ( D 'FEG( H 0 2 F E 2 01 I : % 1 D ( D 'FEG( H 0 2 F E 2 0 1 : ! & ' ( ) ( * +-, . ) / 0 1 0 2 ) 2 ' , . ) / 0 , .)/ 0 , .)/ 0 (0 0 * 3 (* ) (2 ' * ' ' / * +(' 4 * ' ' / * + (' 4 * ' ' / * +(' 4 % 5 687 9 : % " 5 6;7 ! : % $ 5 687 ! :
Fig. 6. Normalized efficiences of p-i-n micromorph solar cells on glass substrate For the p-i-n micromorph tandem solar cell, the spectral response measurements show that it is the microcrystalline (bottom) cell that is damaged after the proton irradiation (Fig. 7). An explanation for this could be found in the different thicknesses of the amorphous and microcrystalline layers of the tandem micromorph cell. As the microcrystalline layers (bottom cell) are about 10 times thicker than the amorphous layers (top cell), there is a higher probability to find radiation-induced damages located at some place along the collection path within the microcrystalline layers. The fact that amorphous material has originally a lot of internal defects and that these solar cells are designed to work with these defects (e.g. by having a higher internal field) could also explain that amorphous layers are much more radiation-resistant than microcrystalline layers.
Relative spectral response [a. u.]
CONCLUSIONS µc-Si:H cell
Wavelength [nm] Fig. 7. Relative spectral response [a. u.] versus wavelength [nm] for the p-i-n micromorph cell (dotted line = measurement after proton irradiation) The capacity of microcrystalline solar cells to recover after thermal annealing was a surprise for us. It is possibly due to the presence of hydrogen within these plasma-deposited microcrystalline layers. The micromorph cells of the first irradiation experiment (fig. 6) have been exposed a second time to the exactly same proton irradiation. After this second bombardment, we have annealed the samples at significantly lower temperatures (70°C, 100°C and 130°C, each annealing step during 10 hours). Experimental results of the same two samples are illustrated in Fig. 8. It shows that after annealing at lower temperatures (70°C, 100°C and 130°C) the degradation due to proton bombardment could be partly recovered. We expect that longer annealing times at temperatures around 70 to 100°C may allow the full recovery of the degradation. It is likely that a steady state will be reached in space, where simultaneous degradation and annealing come to a balance.
P KL P KJ J KO c J KN ηf g h i j k ηf g l m k J KM J KL J KJ
\ n S n R o S p [ ] o ] [ \ d;P \ n Sn R o Sp [ ] o ] [ \ d L Q R S T S U VXW Y T Z [ \ [ ] T ] R W Y T Z [ W YTZ [ W YTZ [ S[ [ U ^ SU T S] R U R R Z U VSR _ U R R Z U VSR _ U R R Z U VSR _ ` J ab c PJ d PJ J ab c PJ d Pe J ab c PJ d
Fig. 8. Normalized efficiencies of p-i-n micromorph solar cells on glass substrates
Up to now, we have manufactured different prototypes of SOLANT (SOLar cell – ANTenna module) using a-Si:H solar cells. Radiation hardness of thin-film amorphous silicon solar cells is excellent, but they have a relatively low power to surface ratio. The use of micromorph tandem solar cells, which hold the promise of significantly higher efficiencies (up to 10 % steady-state space efficiency), could result in a much better power to surface ratio. Although these micromorph solar cells showed an important loss of efficiency immediately after the proton irradiation experiment, they could also be used in space applications. This is due to the fact that the operating temperature of space cells can be up to 100°C (modules without heat-reflecting cover layers) and we suppose that an extended annealing at this temperature could recover the full degradation. The thermal history of the solar modules in space is therefore very important. Further research should de done to clarify the interaction between degradation and recovery as a function of temperature. The work reported was carried out in part under contract No. 12879/98/NL/NB ot the European Space Agency. REFERENCES  M. Tanaka et al., “Microstrip antenna with solar cells for microsatellites”, Electronics Letters, 31, 1995, pp. 5-6  S. Vaccaro et al., “Integration of antennas and solar cells for satellite communications”, AP 2000, Davos  S. Vaccaro et al., “Integrated solar panels antennas”, Electronics Letters, 36, 2000  S. Guha et al., “Amorphous silicon alloy solar cells for nd space applications”, 2 WCPEC, Wien, Austria, 1998  G. J. Vendura et al., “Irradiation and annealing of nd amorphous silicon space cells”, 2 WCPEC, 1998  G. Oomen et al., “The effects of extremely high nd radiation fluxes on amorphous silicon alloy cells”, 2 WCPEC, 1998  J. Kuendig et al., “Effect of proton irradiation on the characteristics of different types of thin-film silicon solar th cells”, 16 EPVSEC, 2000  N. Wyrsch et al., “Development of inverted micromorph nd solar cells”, 2 WCPEC, 1998, pp. 467-471  J. Meier et al., “Microcrystalline and micromorph thinnd film silicon solar cells”, 2 WCPEC, 1998, pp. 375-380  J. Meier et al., “Microcrystalline/micromorph silicon thin-film solar cells prepared by the VHF-GD technique”, PVSEC 11, 1999  H. Schock, K. Bogus, "Development of CIS solar cells nd for space applications", 2 WCPEC, 1998, pp. 3586-3589  H. Curtins, N. Wyrsch, A. Shah, "High rate deposition of amorphous hydrogenated silicon: effect of plasma excitation frequency", Electr. Lett. 23, (1987), p. 228-230